#------------------------------------------------------------------------------
#$Date: 2016-03-26 01:29:34 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180103 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/01/7100186.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7100186
loop_
_publ_author_name
S.R.Miller
P.A.Wright
C.Serre
T.Loiseau
J.Marrot
G.Ferey
_publ_section_title
;
A microporous scandium terephthalate, Sc₂(O₂CC₆H₄CO₂)₃,
with high thermal stability
;
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/b506677h
_journal_year                    2005
_chemical_formula_sum            'C24 H12 O12 Sc2'
_chemical_formula_weight         582.26
_space_group_IT_number           70
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-F 2uv 2vw'
_symmetry_space_group_name_H-M   'F d d d :2'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   8.7550(3)
_cell_length_b                   20.7786(7)
_cell_length_c                   34.4075(13)
_cell_measurement_temperature    293(2)
_cell_volume                     6259.3(4)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    1.236
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Orthorhombic' changed to 'orthorhombic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'F d d d'
_cod_database_code               7100186
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+3/4, -y+3/4, z'
'-x+3/4, y, -z+3/4'
'x, -y+3/4, -z+3/4'
'x, y+1/2, z+1/2'
'-x+3/4, -y+5/4, z+1/2'
'-x+3/4, y+1/2, -z+5/4'
'x, -y+5/4, -z+5/4'
'x+1/2, y, z+1/2'
'-x+5/4, -y+3/4, z+1/2'
'-x+5/4, y, -z+5/4'
'x+1/2, -y+3/4, -z+5/4'
'x+1/2, y+1/2, z'
'-x+5/4, -y+5/4, z'
'-x+5/4, y+1/2, -z+3/4'
'x+1/2, -y+5/4, -z+3/4'
'-x, -y, -z'
'x-3/4, y-3/4, -z'
'x-3/4, -y, z-3/4'
'-x, y-3/4, z-3/4'
'-x, -y+1/2, -z+1/2'
'x-3/4, y-1/4, -z+1/2'
'x-3/4, -y+1/2, z-1/4'
'-x, y-1/4, z-1/4'
'-x+1/2, -y, -z+1/2'
'x-1/4, y-3/4, -z+1/2'
'x-1/4, -y, z-1/4'
'-x+1/2, y-3/4, z-1/4'
'-x+1/2, -y+1/2, -z'
'x-1/4, y-1/4, -z'
'x-1/4, -y+1/2, z-3/4'
'-x+1/2, y-1/4, z-3/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sc Sc 0.3750 0.3750 0.114326(4) 0.01379(5) Uani 1 2 d S . .
O1 O 0.24144(8) 0.41664(4) 0.07046(2) 0.03527(17) Uani 1 1 d . . .
O2 O 0.24534(9) 0.41578(5) 0.15743(2) 0.0486(3) Uani 1 1 d . . .
O3 O 0.50514(9) 0.45836(3) 0.11471(3) 0.0428(2) Uani 1 1 d . . .
C1 C 0.10238(10) 0.43029(5) 0.06762(2) 0.02959(18) Uani 1 1 d . . .
C2 C 0.04973(10) 0.46628(6) 0.03254(2) 0.0331(2) Uani 1 1 d . . .
C3 C 0.15381(11) 0.48582(9) 0.00464(4) 0.0537(4) Uani 1 1 d . . .
H3 H 0.2570 0.4764 0.0076 0.064 Uiso 1 1 calc R . .
C4 C -0.10378(11) 0.48043(9) 0.02788(4) 0.0544(4) Uani 1 1 d . . .
H4 H -0.1738 0.4673 0.0466 0.065 Uiso 1 1 calc R . .
C5 C 0.6250 0.48638(5) 0.1250 0.0293(2) Uani 1 2 d S . .
C6 C 0.6250 0.55826(5) 0.1250 0.0326(3) Uani 1 2 d S . .
C7 C 0.48851(12) 0.59144(4) 0.12457(6) 0.0559(4) Uani 1 1 d . . .
H7 H 0.3966 0.5691 0.1237 0.067 Uiso 1 1 calc R . .
O1W O -0.04002(12) 0.03800(4) 0.03600(6) 0.150 Uiso 0.032(5) 1 d PR . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sc O2 2.0510(7) 2 ?
Sc O2 2.0510(7) . ?
Sc O3 2.0733(7) . ?
Sc O3 2.0733(7) 2 ?
Sc O1 2.0962(6) 2 ?
Sc O1 2.0962(6) . ?
O1 C1 1.2538(10) . ?
O2 C1 1.2487(10) 11_454 ?
O3 C5 1.2511(9) . ?
C1 O2 1.2488(10) 11_454 ?
C1 C2 1.4928(10) . ?
C2 C3 1.3846(12) . ?
C2 C4 1.3851(13) . ?
C3 C4 1.3914(13) 17_565 ?
C3 H3 0.9300 . ?
C4 C3 1.3913(13) 17_565 ?
C4 H4 0.9300 . ?
C5 O3 1.2511(9) 11_554 ?
C5 C6 1.4936(15) . ?
C6 C7 1.3797(12) 11_554 ?
C6 C7 1.3797(12) . ?
C7 C7 1.3947(19) 8_554 ?
C7 H7 0.9300 . ?
